Download presentation

Presentation is loading. Please wait.

Published byKimberly Baily Modified over 2 years ago

1
Fibre Volume Fraction and Laminate Thickness

2
How much fibre…?

3
How much reinforcement? Weight fraction Used in manufacture. May refer to fibre or resin - 'GRP' manufacturers will specify a glass content of (e.g.) 25 wt%; a prepreg supplier might give a resin content of 34 wt%. Volume fraction Used in design to calculate composite properties. Almost always refers to fibre content.

4
Weight fraction volume fraction conversion For the special case of a two-component composite (eg fibre and matrix):

5

6
Maximum fibre volume fraction A composite cannot contain 100% fibre. Maximum volume fraction could be achieved only if unidirectional fibres are hexagonally close packed - ie all fibres are touching.

7
Maximum fibre volume fraction The triangular unit cell has area 3 R 2. The unit cell contains an area of fibre (three 60 o segments) equal to R 2 / 2 2R 3R

8
Maximum fibre volume fraction In a unidirectional fibre composite, the fibre area fraction is the same as the fibre volume fraction, so:

9
Maximum fibre volume fraction Theoretically, a unidirectional fibre composite could have V f 90%. In practice, fibres cannot be perfectly aligned. Maximum volume fraction depends both on the fibre form and method of manufacture - for a unidirectional fibre composite: V f 60-70%.

10
Maximum fibre volume fraction For other forms of reinforcement, maximum volume fraction also depends on the detailed arrangement of the fibres. The following values are typical: stitched non-crimp0.6 woven fabric random (chopped strand mat)

11
How much fibre? Commercial reinforcements are characterised by their areal weight (A w ). This is simply the weight (usually given in g) of 1 m 2 of the reinforcement. A w depends on many factors - fibre density, tow or bundle size, weave style, etc. A w may range from 50 g/m 2 or less (for lightweight surfacing tissues), up to more than 2000 g/m 2 for some heavyweight non-crimp fabrics.

12
Laminate thickness The thickness of a composite laminate depends on the amount of reinforcement and the relative amount of resin which has been included. For a given quantity of reinforcement, a laminate with a high fibre volume fraction will be thinner than one with a lower fibre volume fraction, since it will contain less resin.

13
Laminate thickness fibre matrix high matrix content low fibre content = thick laminate low matrix content high fibre content = thin laminate Two laminates, both containing 5 plies of reinforcement:

14
Laminate thickness Fibre volume fraction is thus inversely proportional to laminate thickness. If the fibre content and laminate thickness are defined, we can calculate the fibre volume fraction: If the fibre content and volume fraction are defined, we can calculate the laminate thickness:

15

16

17
Example calculations Example calculations 1. What will be the thickness of a laminate consisting of 2 layers of 450 g/m 2 chopped strand mat if a resin to glass ratio (by weight) of 2:1 is used? 2. What fibre volume fraction is achieved if 3 layers of 800 g/m 2 glass woven roving are compression-moulded to a thickness of 2 mm?

18
Rules of Mixture for Elastic Properties

19
'Rules of Mixtures' are mathematical expressions which give some property of the composite in terms of the properties, quantity and arrangement of its constituents. They may be based on a number of simplifying assumptions, and their use in design should tempered with extreme caution!

20
Density For the special case of a fibre-reinforced matrix: since V f + V m = 1

21
Rule of mixtures density for glass/epoxy composites f m

22
Micromechanical models for stiffness

23
Unidirectional ply Unidirectional fibres are the simplest arrangement of fibres to analyse. They provide maximum properties in the fibre direction, but minimum properties in the transverse direction. fibre direction transverse direction

24
Unidirectional ply We expect the unidirectional composite to have different tensile moduli in different directions. These properties may be labelled in several different ways: E 1, E || E 2, E

25
Unidirectional ply By convention, the principal axes of the ply are labelled 1, 2, 3. This is used to denote the fact that ply may be aligned differently from the cartesian axes x, y, z

26
Unidirectional ply - longitudinal tensile modulus We make the following assumptions in developing a rule of mixtures: Fibres are uniform, parallel and continuous. Perfect bonding between fibre and matrix. Longitudinal load produces equal strain in fibre and matrix.

27
Unidirectional ply - longitudinal tensile modulus E 1 = E f V f + E m ( 1-V f ) Note the similarity to the rules of mixture expression for density. In polymer composites, E f >> E m, so E 1 E f V f

28
This rule of mixtures is a good fit to experimental data (source: Hull, Introduction to Composite Materials, CUP)

29
Unidirectional ply - transverse tensile modulus The simplified model lumps fibre and matrix together, and assumes that both components experience the same stress: 2 2 LfLf LmLm or

30
If E f >> E m, E 2 E m / (1-V f ) Note that E 2 is not particularly sensitive to V f. If E f >> E m, E 2 is almost independent of fibre property:

31
carbon/epoxy glass/epoxy The transverse modulus is dominated by the matrix, and is virtually independent of the reinforcement.

32
The transverse rule of mixtures is not particularly accurate, due to the simplifications made - Poisson effects are not negligible, and the strain distribution is not uniform: (source: Hull, Introduction to Composite Materials, CUP)

33
Generalised rule of mixtures for tensile modulus E = L o E f V f + E m (1-V f ) L is a length correction factor. Typically, L 1 for fibres longer than about 10 mm. o corrects for non-unidirectional reinforcement:

34

35

36

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google